INNOVATIVE PROCESS MODEL OF TI-6AL-4V · PDF fileINNOVATIVE PROCESS MODEL OF TI-6AL-4V...
Embed Size (px)
Transcript of INNOVATIVE PROCESS MODEL OF TI-6AL-4V · PDF fileINNOVATIVE PROCESS MODEL OF TI-6AL-4V...
INNOVATIVE PROCESS MODEL OF TI-6AL-4V ADDITIVE
LAYER MANUFACTURING USING COLD METAL
P.M. Sequeira Almeida1*
, S. Williams1**
1 Welding Engineering Research Centre (WERC), Cranfield University
MK43 0AL, United Kingdom
New approaches to modern manufacture have emerged from Additive Layer Manufacturing
(ALM) technologies over the last 25 years. These approaches provide form, fit and function to
a wide range of metallic alloys and components. Wire + Arc Additive Layer Manufacture
(WAALM) has gained the interest of the research community in recent years due to its high
deposition rate and efficiency (100%). The technique has been presented to the aerospace
manufacturing industry as a unique low cost solution for large structural components
manufacture. With this process product development time, capital investment and Buy-to-
Fly ratios can be significantly improved. One of the greatest challenges of WAALM systems
is the control algorithms needed to predict optimum welding parameters in order to achieve a
specific target wall width/height requirement, and maximum deposition efficiency. This paper
describes a process model for multilayer Ti-6Al-4V deposition using the Gas Metal Arc
Welding based process of Cold Metal Transfer. The process model is based on a Systematic
Experimental Approach carried out using a regression analysis. The mathematical
relationships obtained are ready to use in future large scale intelligent WAALM controllers.
Keywords: Wire + Arc Additive Layer Manufacture (WAALM), Additive Layer Manufacturing
(ALM), Cold Metal Transfer (CMT), Ti-6Al-4V, Buy-to-Fly, Systematic Experimental
Approach (SEA), High Deposition Rate.
The economical gains and environmental impact of innovative Wire + Arc Additive Layer
Manufacture (WAALM) solutions over traditional manufacturing technologies for large scale
manufacture, is directly dependent on the processing speeds, and therefore on the deposition
rates capability. The practice becomes even more ingrained for cost effective production of
high value components for aerospace industry applications, such as Ti-6Al-4V, where soaring
Material Utilization Factors (MUFs) of less than 15%, normally provided by traditional
forging/machining routes, need to be considered . For that reason, several state of the art
wire based ALM solutions are being investigated at Cranfield University in the Welding
Engineering Research Centre. In the present study an out-of-chamber cold wire fed Gas
Tungsten Arc Welding (GTAW) solution was utilised for the fabrication of a large structural
Ti-6Al-4V component. The independent control of the wire feed speed (WFS) over the net arc
power, and vice versa, resulted in a precise control over the molten pool dimensions, and the
amount of metal transferred into it. The as welded component has demonstrated the enormous
potential of the GTAW based system for the manufacture of large and high quality structural
components. However, while geometrical accuracy and surface finish are two of the main
attributes of the former system, the main drawback is still the substantial lower deposition rate
capability, when compared with a Gas Metal Arc Welding (GMAW) based process.
Generally, WAALM deposition rate capabilities can go up to 1kg/h for cold wire fed GTAW,
while several kilograms per hour can be achieved by utilising a GMAW based system.
However poor welding conditions are in general attained and reproduced by gaseous titanium
arcs. In particular Direct Current Electrode Positive (DCEP)-GMAW of titanium and titanium
alloys is mainly characterized as unstable, uncontrollable and very prone to severe spattering
conditions, which reduces the weld bead quality and overall process efficiency. The nature of
the erratic titanium arc behaviour is caused by a dynamic cathode spot relocation mechanism
observed on the active cathodic region, the molten pool.
Various approaches have been examined to overcome these problems. Recently Zhang
and Li  proposed a modified active control to improve the robustness of the One Droplet
Per Pulse (ODPP) metal transfer mechanism of titanium and titanium alloys on GMAW-P
base systems. Additionally Shinn, et al. have successfully reported a hybrid approach to
confine the cathode spot relocation and suppress spatter, by utilising a low power continuous
wave Nd:YAG laser beam with a minimum power of 200W and a spot diameter of 0.6mm
and a GMAW-P system on Ti-6Al-4V deposition.
In the present study an innovative GMAW based solution, namely Cold Metal Transfer
(CMT), has been investigated for its suitability for high deposition rate ALM of Ti-6Al-4V.
CMT is a modified GMAW variant based on a controlled dip transfer mode mechanism. The
process delivers excellent quality, lower thermal heat input, and nearly spatter free weld. The
CMT process overcomes common difficulties encountered during conventional short
circuiting GMAW such as unstable process behaviour and severe spatter formation . The
pioneering and key determining difference when compared with conventional GMAW is that
for the first time the mechanical motion of the wire is directly incorporated into the electrical
process control. The reciprocated wire feeding system is synchronized with a high speed
digital control that senses the arc length, short circuiting phase and thermal input transferred
to the weld . When the wire moves forward and dips in the molten pool the digital control
senses the voltage drop and that a short circuiting phase occurred and the current is then
reduced to a significantly lower level. A feedback signal returns to the wire feeder in order to
reverse the feeding direction. Then the wire back-drawing force assists the liquid bridge
fracture  and the droplet detachment takes place. The metal transfer occurs by surface
tension at near zero current. The arc ignition is initiated by an initial pulse of current that re-
establishes the arc length and pre-melts a considerable amount of the wire volume. It should
be noted that the movement of the motor of the driving unit is based on optimized arc
characteristics rather than predefined times or speeds .
A key element of the successful application of WAALM is the development of a process
model that enables the prediction of weld bead geometry from the process parameters.
Distinct mathematical approaches have been employed for this spanning from statistical to
numerical methods. Factorial designs [8, 9], linear regression [10, 11], response surface
methodology [12-14], artificial neural networks (ANNs) [15, 16], taguchi method [17-21],
controlled random search (CRS), or combinations of two techniques  have been reported.
In this paper a process model for multilayer Ti-6Al-4V WAALM utilising the CMT is
described. The process model is based on a comprehensive Systematic Experimental
Approach (SEA) carried out using a regression analysis. Optimum welding conditions are
obtained in order to achieve a specified target effective wall width, height, and deposition
rates. The preliminary mathematical relationships obtained are ready to use in future large
scale intelligent WAALM controllers, and presently undergoing an optimization process.
The experiments were conducted on Ti-6Al-4V substrates with dimensions 170 mm x 170
mm x 8mm. The chemical composition of the alloy (in wt. %) is provided in Table 1. The
transus for this composition is approximately 995C. Ti-6Al-4V wire diameters were 0.9 and
1.2mm spool with the chemical composition also shown in Table 1.
Table 1. Chemical composition of Ti-6Al-4V including alloying elements and impurities content (wt. %).
Alloy Al Mo V Cr Fe C Si H N O Ti
Ti-6Al-4V1 6.28 - 4.15 - 0.15 0.03 - 0.01 0.04 0.12 Balance
Ti-6Al-4V2 6.14 - 3.96 - 0.18 0.02 - 0.001 0.011 0.14 Balance
1 chemical composition for the substrate; 2 chemical composition for the 0.9 and 1.2mm wires.
Four state of the art high deposition rate WAALM systems, namely CMT, GTAW; using
two variants Pulsed (GTAW-P) and Gas Tungsten Constricted Arc Welding (GTCAW); and
DCEP-GMAW, were utilised during this investigation to lay down single and multilayer Ti-
6Al-4V deposits. Firstly the DCEP-GMAW system was used for high deposition rate single
bead on plate experiments in order to assess the welding arc stability, the quality of the
deposited beads and reproducibility of the process. The same procedure was subsequently
applied to the CMT system. In the latter the impact of different shielding gas mixtures on the
resultant Ti-6Al-4V single bead microstructures, containing Ar/He (30%, 50% and 70%), was
investigated. Additionally, a series of Ti-6Al-4V multilayer walls (10 layers), were deposited
in a linear sequence utilising both the CMT and GTAW-P systems in order to assess the
deposits grain size distribution and morphology, as represented schematically in Fig. 1.
Finally, and for the first time the InterPulse GTCAW system was employed as a heat source